Passivation is a must after every pickling operation process.
Next apply K-2 passivation solution and leave it for 20-25 minutes.
Finally clean the surface thoroughly with water.
HOW TO APPLY K - 2 PASTE
1. First remove oil, dirt etc. with SI 56
degreaser. Add 50 - 75 gm/lit. in water & stir to dissolve. Wipe
S.S. surface with cotton cloth or spray or soak for 10 min. Wash
with water and allow to dry.
(Steps 1 & 5 can be avoided for K-2 PASTE on weld seam
2. K-2 PASTE is applied on weld seam & surrounding areas with a
nylon bristled plastic brush OR
K-2 Spray is sprayed on S.S. surface with plastic pressurized
spray bottle or pump
OR K-2 Dip is used to dip S.S. components in a plastic tank or
circulated in pipeline with pump.
Application Temp. = Between 25 - 35 deg. C .
If temp. is less than more time may be required and if temp. is
more than uneven processing may result. So, cool SS equipment by
keeping its in shade & not directly under the sun.
3. Keep K-2 product for 10 - 45 minutes depending on
contamination & scale. ( K-2 PASTE generally kept for 10 - 30
min. and K-2 Spray generally kept for 30 - 45 min. )
4. Wipe the weld seam lightly with plastic brush or cloth & wash
with water thoroughly & allow to dry.
5. Spray or Dip in K-2 Passivation or K-2 Biopassive solution &
leave it for 10- 20 minutes. Rinse with water thoroughly.
For Passivating Mirror Bright Buffed /
Polished SS Areas,
THE BELOW STEPS WILL NOT AFFECT SHINE OF MIRROR
BRIGHT BUFFED / POLISHED SS AREAS AND PROVIDE CONTAMINATION &
STERILE PARTICLE FREE PASSIVATED SS SURFACE.
1 First apply K-2 PASTE on weld seam & surrounding areas with a
nylon bristled plastic brush. After 10 to 30 min. wipe with
cloth or plastic brush & wash with water thoroughly.
( Application of K-2 PASTE ensures that black & red spots do not
come on & near weld seams area as generally observed some days
after bright buffing. )
2 Complete usual bright buffing / polishing procedure to make
surface mirror bright & shiny.
( If SS eqpt. or pipe is already bright buffed or polished then
discard Steps 1 & 2 and start directly with Step 3 )
3 Remove oil, dirt, buffing compounds etc. with "SI 56" -
sulphur free degreaser.
Add 50 - 75 gm/lit. in water ( 1 kg SI 56 in 15 – 20 Lit. water
) & stir to dissolve. Wipe S.S. surface with cotton cloth or
pressurized spray for 2 - 5 min. or soak small parts for 10 min.
Wash with water properly.
4 Spray or Dip in K-2 passivation or K-2 Biopassive & leave it
for 15 - 25 minutes. Then, rinse with water thoroughly.
"SURFACE INNOVATORS " PROVIDES EQUIPMENTS & ACCESSORIES FOR
SAFE, IN-HOUSE PICKLING & PASSIVATION FOR ALL TYPES OF JOBS.
PRODUCT APPROVED BY I.I.T. (BOMBAY) UNDER ASTM – A380
ASTM = American Standards of Testing Materials